Research Article | Open Access
Siti Zulaikha Mazlan, Faszly Rahim, Sharina Abu Hanifah, "Facile Synthesis of Magnetic Copolymer Microspheres Based on Poly(glycidyl methacrylate-co-N-isopropylacrylamide)/Fe3O4 by Suspension Photopolymerization", International Journal of Polymer Science, vol. 2014, Article ID 591898, 7 pages, 2014. https://doi.org/10.1155/2014/591898
Facile Synthesis of Magnetic Copolymer Microspheres Based on Poly(glycidyl methacrylate-co-N-isopropylacrylamide)/Fe3O4 by Suspension Photopolymerization
Magnetic copolymer based on poly(glycidyl methacrylate-co-N-isopropylacrylamide) microspheres was prepared by 2,2-dimethoxy-2-phenylacetophenone- (DMPP-) photo initiated and poly(vinyl alcohol)- (PVA-) stabilized single step suspension photopolymerization. The effect of chemical interaction, morphology, and thermal properties by adding 0.1% w/v Fe3O4 in the copolymer was investigated. Infrared analysis (FTIR) showed that (C=C) band disappeared after copolymerization, indicating that the magnetic copolymer microspheres were successfully synthesized and two important bands at 908 cm−1 and 1550 cm−1 appear. These are associated with the epoxy group stretching of GMA and secondary amide (N–H/C–H) deformation vibration of NIPAAm in magnetic microspheres. The X-ray diffraction (XRD) result proved the incorporation of Fe3O4 nanoparticles with copolymer microspheres as peak of Fe3O4 was observed. Morphology study revealed that magnetic copolymer exhibited uniform spheres and smoother appearance when entrapped with Fe3O4 nanoparticles. The lowest percentage of Fe3O4 nanoparticles leached from the copolymer microspheres was obtained at pH 7. Finally, thermal property of the copolymer microspheres was improved by adding a small amount of Fe3O4 nanoparticles that has been shown from the thermogram.
Magnetic polymer microspheres with core-shell morphology combining a polymer material and inorganic nanoparticles give unique properties of both materials which have been investigated extensively in various fields, such as isolation biological compound, drug delivery, and protein purification, particularly in sorbent to remove metal ions and enzyme immobilization [1–4]. This is due to their multifunctional properties such as small and uniform size, various functional groups on the surface, and large surface area [5, 6]. Moreover, considering their magnetic properties, this magnetic polymer can easily separate and provide not only better physical and chemical stability, but also superior biological compatibility as reported . The presence of polymer material provides the magnetic nanoparticle with high abundance of functional group through copolymerization and chemical modification step. These magnetic polymer microspheres capable to ensure a strong magnetic response and polymeric material can provide favourable functional groups and ability to protect nanoparticles aggregation . Therefore, many polymer materials such as poly(styrene-glycidyl methacrylate) magnetic have been prepared in which Fe3O4 was modified with polyethylene glycol (PEG) and oleic acid (OA) . The results reveal that the polymer is porous with high magnetic contents. Lan et al. 2013  synthesized hyaluronic acid-supported magnetic microspheres utilized as adsorbent for heavy metal removal. The resultant microspheres showed superparamagnetic behavior, which made these adsorbents magnetically separable after the adsorption performance.
Glycidyl methacrylate (GMA) based copolymers have benefit because of the presence of reactive epoxy group. Epoxy groups have unique capability because they can be easily modified to a variety of functional groups such as aldehyde, aliphatic primary amino, and diazotizable primary aromatic groups . Furthermore, polymers with epoxide groups offer numerous functionalization possibilities in mild reaction conditions . It is suitable for prospective immobilization of enzymes and other proteins and nucleic acids . N-isopropylacrylamide (NIPAAm) acts as a second monomer in this system. It is one of the most well-known temperature-sensitive polymers, exhibiting a low critical solution temperature (LCST) at 32°C which provides hydrogel with the possibility to have high swelling degrees at low temperatures and shrink at high temperatures . Thermoresponsive swelling behaviour can be designed and utilized in several advanced applications as reported by Kali et al. 2013 using novel amphiphilic conetworks (APCN) consisting of thermoresponsive poly(N-isopropylacrylamide) cross-linked by hydrophobic methacrylate-telechelic polyisobutylene. This study revealed the LCST of these conetworks decreases to the range of 25–28°C in comparison with 34.1°C for the homopolymer network of poly(NIPAAm). As a consequence, significant decreases of swelling degree in water between 20 and 35°C are observed . In addition, hydrophilic/hydrophobic balance in the NIPAAm unit results from hydrophilic (amide group) and hydrophobic (isopropyl group) regions of poly(NIPAAm). Below the LCST, hydrogen bonding between hydrophilic segments and water molecules is dominant which can lead to enhancing dissolution or swelling in water. As the temperature increases, hydrophobic interactions among the hydrophobic segments become stronger, while hydrogen bonding becomes weaker, resulting in shrinking of the hydrogels .
Thus far, several conventional procedures have been proposed for the encapsulation of iron oxide nanoparticles in polymer shells including solvent evaporation and heterogeneous polymerizations such as suspension, emulsion, and dispersion/precipitation polymerization [14–17]. Upon completion of polymerization, iron oxide nanoparticles are evenly distributed or could be within the pores of the polymer . Recently, researchers had prepared magnetic poly(vinyl acetate-divinylbenzene) microspheres using modified suspension polymerization. As a result, they can control beads size within 10 μm, but the size distribution was still wide and a part of the microspheres sphericity was altered. In the case of products that were prepared by emulsion polymerization, there are still some drawbacks such as weak magnetic responsiveness, low particle yield, and severe flocculation of microspheres. Therefore, suspension radical polymerization can be considered to be the most favorable approach in the preparation of magnetic monodisperse microspheres [1, 17]. Furthermore, suspension photopolymerization technique was carried out either without or with a low amount of cross-linking agent .
In view of these problems, this work proposes a new method of suspension photopolymerization that offers a rapid and straightforward technique of copolymerization. The effects of incorporating iron oxide (Fe3O4) nanoparticles into the copolymer microspheres also were investigated using several physical analyses. The analyses include phase transition of the resultant magnetic copolymer that was measured by differential scanning calorimetry (DSC), morphology property using scanning electron microscopy (SEM), and iron oxide (Fe3O4) nanoparticles leached from the copolymer microspheres and was also determined by atomic absorption spectroscopy (AAS).
Glycidyl methacrylate, GMA (Sigma-Aldrich), N-isopropylacrylamide, and NIPAAM (Sigma-Aldrich) were stored in a refrigerator and at room temperature until use, respectively. Iron oxide, Fe3O4, 20–50 nm (Sigma-Aldrich), 2,2-dimethoxy-2-phenylacetophenone, DMPP (Sigma-Aldrich), poly(vinyl alcohol), and PVA (Sigma-Aldrich) were selected as the photo initiator and stabilizer, respectively. The cross-linker, ethylene glycol dimethacrylate (EGDMA), was obtained from Sigma-Aldrich. Deionised water was used for making the aqueous solution during the experiment. All chemicals were used without purification.
2.2. Synthesis of Magnetic Copolymer
The magnetic copolymer GN73 was prepared via suspension photopolymerization as described below. A mixture was comprising 70% v/v GMA, 30% w/v NIPAAM, 0.1% w/v Fe3O4, and 600 µL of EDGMA in a sample bottle followed by 5 mL of 1% w/v PVA and 1.6% w/v DMPP added to a sample bottle. This mixture was sonicated at 37°C for 10 min to assure adequate dispersion . The photo curing of the final mixture was performed under ultraviolet (UV) radiation in a UV box (RS Ltd.) containing four units of 60 watt UV lamps. The irradiation was carried out for 10 min under a nitrogen atmosphere . After completion of polymerization, the copolymer microspheres were centrifuged at 5000 rpm for 10 min to remove the suspended medium. The polymerization reaction led to the formation of milky magnetic copolymer (GMA-NIPAAM) microspheres which were resuspended in 10 mL of ethanol and centrifuged again under similar conditions. The ethanol wash step was repeated three times to complete removal of unreacted monomers. Finally, magnetic copolymer GN73 microspheres were resuspended in 10 mL of deionised water and stored at room temperature until use . All the steps were repeated to obtain the copolymer without magnetic particles (GN73).
2.3. Characterization Techniques
Functional groups in the magnetic copolymer GN73 were determined using Fourier transform infrared (FTIR, Perkin-Elmer Spectrum BX) at normal transmission mode and wavelength from 4000 to 370 cm−1 at 2 cm−1 resolution. Each sample (powder form) was analyzed in a form of KBr disc. The phase composition and structure of the magnetic copolymer GN73 were determined by X-ray powder diffraction (XRD) using a D8-Advance Bruker AXS (monochromated Cu Kα radiation = 1.5418 Å). Typically, the diffractogram was recorded in a 2θ range of 3–80°C. The phase transition behaviour of magnetic copolymer GN73 was determined by using DSC (Perkin Elmer model DSC-7). About 4 mg of magnetic copolymer GN73 microspheres was placed in an aluminium pan and sealed tightly using aluminium lid. Thermal analysis was performed from 0 to 220°C under dry nitrogen atmosphere with a flow rate of 5 mL/min at heating rate of 10°C/ minutes. Morphology and size of the magnetic copolymer GN73 microspheres were studied using SEM (Zeiss Supra 55VP, Germany). Magnetic copolymer GN73 microspheres were dried at room temperature, coated with a thin layer of platinum (about 100 Å) in vacuum, and observed at 10,000x magnification. In this study, three types of leaching medium were used: 50% acetic acid solution (pH 3.0), 50 mM phosphate buffer solution (pH 7.0), and 50 mM sodium citrate/NaOH buffer solution (pH 12.0). Approximately, 250 mg of the magnetic copolymer was placed in a test tube containing 10 mL of a leaching medium and shaken with a rotary shaker for 24 h. Then, the amount of iron oxide (Fe3O4) nanoparticles that leached out into the medium was determined by an atomic absorption spectroscopy (AAS 5EA, Carl Zeiss Technology, Zeiss Analytical Systems, Germany).
3. Results and Discussion
3.1. Preparation of Magnetic Microspheres
The proposed reaction for the formation of magnetic polymer microspheres via suspension photopolymerization is displayed in Figures 1(a) and 1(b). Initially, iron oxide (Fe3O4) nanoparticles and monomers (GMA and NIPAAM) were restricted in suspension droplet, which was stabilized by PVA and EGDMA. When the mixture was polymerized by the UV irradiation, the miscibility of monomer mixture and iron oxide (Fe3O4) nanoparticles resulted in a phase separation. However, before the iron oxide (Fe3O4) nanoparticles totally escaped from the polymer phase, the viscosity became high enough to prevent the phase separation. Hence, the magnetic microspheres were obtained after only 10 min of UV irradiation . Miscibility monomer depends either on specific interactions or on intermolecular repulsion. Since there are epoxy ring in GMA chain and active hydrogen in the side chain of NIPAAM, they are leading to the formation of intermolecular interaction as shown in Figure 1(b).
3.2. FTIR Analysis
The chemical composition of the magnetic copolymer was assessed using FTIR spectroscopy. Figure 2(a) illustrates the FTIR spectra of the copolymer GN73 and magnetic copolymer GN73 is shown in Figure 2(b). Both spectra show important characteristic peak at 908 cm−1, indicating the presence of epoxy group in copolymer. Besides, the spectra show absorption peaks at 1733 cm−1 (C=O carbonyl vibration) and two peaks at 1670 cm−1 and 1550 cm−1 correspond to amide I (C=O/C–N) and amide II (N–H/C–H) vibration, respectively, representing the acrylamide vibration of NIPAAm unit. The peak at 1258 cm−1 could be attributed to the stretching vibrations of C–O configuration of GMA. In addition, a new sharp peak was observed at 594 cm−1. It may be due to the Fe–O vibration band of bulk Fe3O4 that is bound in tetrahedral geometry . These results proved that magnetic nanoparticles were successfully entrapped onto the copolymer microspheres by suspension photopolymerization.
3.3. XRD Analysis
The structure of iron oxide in magnetic copolymer was analyzed using X-ray diffraction (XRD) . Diffractogram (Figure 3) shows a diffraction pattern between copolymer GN73 and magnetic copolymer GN73. The XRD patterns of magnetic copolymer GN73 microspheres, as illustrated in Figure 3, did not change distinctly as the copolymer GN73 (a peak at 2θ of about 19.0°) only increases the peak strength. Therefore, it could be demonstrated that iron oxide (Fe3O4) nanoparticles had been successfully incorporated into the copolymer microspheres and GN73 without being destroyed . The XRD patterns of magnetic copolymer GN73 and pure iron oxide (Fe3O4) nanoparticles are shown in Figure 4. The overlap between magnetic copolymer GN73 and iron oxide (Fe3O4) nanoparticles peak proved the existence of iron oxide (Fe3O4) nanoparticles in magnetic copolymer (the diffraction peaks at 2θ of about 18.2°, 21.1°, 30.0°, 37.0°, 45.0°, and 62.5°). It is apparent that the diffraction pattern of the iron oxide (Fe3O4) in copolymer is closed to the standard pattern for crystalline iron oxide . The overlaps show the presence of iron oxide at the spinal structure .
3.4. DSC Analysis
Phase transition behaviour of each sample was analyzed using differential scanning calorimeter (DSC). The Tg of poly(GMA), poly(NIPAAm), copolymer GN73, and magnetic copolymer GN73 was shown in Figure 5. The Tg of poly(GMA) obtained via suspension photopolymerization was 78°C and comparable to the Tg of poly(GMA) by using precipitation polymerization that was 83°C . The Tg value for cross-linked poly(GMA) has increased to 78°C compared to the reported finding, 60°C for poly(GMA) homopolymer without cross-linker. The increase of Tg may be due to cross-linking effect which significantly lowers the mobility of chains. Thus, a higher temperature is needed for promoting chain mobility . In Figure 5(c), the endothermic peak refers to the melting point (Tm) of poly(GMA) around 190°C. Figure 5(d) indicates moisture removal from 60 to 85°C for poly(NIPAAm). The observation was also reported in the poly(NIPAAm) homopolymer that was obtained by radical polymerization . On the other hand, the glass transition temperatures of poly(GMA) and poly(NIPAAm) were 78°C and 136°C, respectively; the Tg values of copolymer GN73 were higher than those of pure components which are 172°C. This is probably caused by higher extent of H-bonding between epoxide group from poly(GMA) and N–H bonds in poly(NIPAAm). Strong hydrogen bond can effectively act as a physical cross-linker, thus reducing segment mobility . Both pure constituents, copolymer GN73 and magnetic copolymer GN73, show a single Tg as shown in Figure 5. It has been shown in the literature  that when the polymers are fully miscible, it will exhibit single glass transition temperatures. Furthermore, the thermogram for magnetic copolymer GN73 exhibited slightly higher Tg (180°C) than copolymer GN73 (172°C) after iron oxide was added to copolymer. As it can be observed, only small amount of magnetite nanoparticles is effective in shifting Tg to the higher value. Therefore, it can be said that there is an enhancement of glass transition in the magnetic copolymer GN73. This kind of observation was also reported by López et al. for their PVA nanocomposite prepared with Co-Fe2O4 nanoparticles. The proposed explanation is related to the restrictions in segment mobility and to the reduction of diffusivity of attacking agents within the polymer matrix, both due to the polymer-filler interactions . The thermal stability of magnetic copolymer GN73 was improved by the presence of magnetite nanoparticles which act as a heat barrier due to the nanoparticle-polymer interaction. The nanoparticle-polymer interaction could be type of adhesive forces. This kind of interaction has been accepted by several authors to exist between magnetite particles and a polymer [33, 34].
3.5. SEM Analysis
Scanning electron microscopy (SEM) is used to elucidate the morphology of the copolymer and the location of pores . Figure 6(a) shows the micrograph of copolymer beads surface without iron oxide nanoparticles, while Figure 6(b) refers to the distribution of beads for magnetic copolymer GN73. From the figures, it can be found that the surface of a bead copolymer GN73 exhibited a loose shallow porous with average pore diameter between 1.0 and 1.5 μm which is estimated based on the SEM micrograph. However, no porous structure was observed in the magnetic copolymer GN73 as seen in Figure 6(b). This finding was constant with previous report in the literature . In comparison with the copolymer GN73, the magnetic copolymer GN73 surface was smoother than copolymer GN73 without magnetic. This is because the iron oxide (Fe3O4) nanoparticles are mostly entrapped within the interstitial spaces of a cross-linked water-insoluble polymer during in situ polymerization of the monomers forming the copolymer . Polymer surfaces are believed to be nonporous because of their very small specific surface area and pores size after substituting iron oxide nanoparticles . As we can see, the magnetic copolymer GN73 has narrow distribution size of beads in the range of 0.34–0.57 μm and dispersed on the surface of the copolymer. This finding reveals that the iron oxide (Fe3O4) nanoparticles were found to be inside and of the microspheres particle surface agree with previous report .
3.6. AAS Analysis
Iron oxide (Fe3O4) is a biocompatible superparamagnetic material that has low toxicity and strong magnetic properties . The relevant kinetic data has been correlated with one or more of the physiochemical factors that include the ionic activity of H+, interaction with OH− or , electrochemical surface reaction, and changes in surface area . Note that the leaching of iron oxide (Fe3O4) nanoparticles was measured in three different media including acetic acid solution (50%, v/v, pH 3.0), phosphate buffer solution (pH 7.0), and sodium citrate/NaOH buffer solution (pH 12.0). The highest iron concentration obtained was 2.048 mg /L in 50% acetic acid solution at pH 3.0. It has been reported  that the optimum pH for dissolving iron oxide is pH 2.5–3.0. In acidic medium, the degree of freedom for poly(NIPAAm) chains was bigger compared to neutral and alkaline medium . So, more iron oxide is eluted at pH 3.0 compared to other pH. Figure 7 shows that the iron oxide (Fe3O4) nanoparticle has the lowest solubility in neutral medium (0.028 mg /L), while the concentration of leached iron oxide (Fe3O4) nanoparticles in alkaline solvent was 0.062 mg/L. It has been previously shown that the iron ions that were entrapped into the polymer matrix can be eluted if there are changes in ionic strength in medium or pH solution .
In summary, magnetic copolymer GN73 microspheres can be rapidly synthesized by suspension photopolymerization in the presence of iron oxide nanoparticles. The synthesized magnetic copolymer GN73 microspheres exhibited narrow distribution size in the range of 0.34–0.57 μm. The pH value of external buffer solution had influenced the leached iron oxide (Fe3O4) nanoparticles from the copolymer microspheres. The result was confirmed by AAS analysis that revealed that the highest amount of leached iron oxide (Fe3O4) occurred in acidic medium. Besides that GN73 copolymer has good miscibility that was led to increase Tg value compared to the homopolymer. The addition of small amount of Fe3O4 has successfully improved the thermal properties of the polymer. This work has potential in biosensor matrix fabrication because of the presence of epoxy ring that can be easily modified to bind with enzyme. Furthermore, a small size of microspheres promotes higher surface area.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
This work was financially supported in part by Research Grants (FRGS/1/2013/ST01/UKM/02/2), (ICONIC-2013-004), and ERGS/1/2011/STG/UKM/02/15 given by Universiti Kebangsaan Malaysia and Ministry of Education.
- D. Horák, E. Pollert, M. Trchová, and J. Kovářová, “Magnetic poly (Glycidyl Methacrylate)-based microspheres prepared by suspension polymerization in the presence of modified La0.75sr0.25mno3 nanoparticles,” European Polymer Journal, vol. 45, no. 4, pp. 1009–1016, 2009.
- S. Bai, Z. Guo, W. Liu, and Y. Sun, “Resolution of (±)-menthol by immobilized Candida rugosa lipase on superparamagnetic nanoparticles,” Food Chemistry, vol. 96, no. 1, pp. 1–7, 2006.
- E. B. Altintaş and A. Denizli, “Efficient removal of albumin from human serum by monosize dye-affinity beads,” Journal of Chromatography B: Analytical Technologies in the Biomedical and Life Sciences, vol. 832, no. 2, pp. 216–223, 2006.
- E. B. Altintaş and A. Denizli, “Monosize poly (glycidyl methacrylate) beads for dye-affinity purification of lysozyme,” International Journal of Biological Macromolecules, vol. 38, no. 2, pp. 99–106, 2006.
- X. Wang, Z. Zhou, and G. Jing, “Synthesis of Fe3O4 poly(styrene-glycidyl methacrylate) magnetic porous microspheres and application in the immobilization of Klebsiella sp. FD-3 to reduce Fe(III)EDTA in a NOx scrubbing solution,” Bioresource Technology, vol. 130, pp. 750–756, 2013.
- S. Chaleawlert-umpon and N. Pimpha, “Preparation of magnetic polymer microspheres with reactive epoxide functional groups for direct immobilization of antibody,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 414, pp. 66–74, 2012.
- J. Zhang, D. Yu, W. Chen et al., “Preparation of poly(styrene-glucidylmethacrylate)/Fe3O4 composite microspheres with high magnetite contents,” Journal of Magnetism and Magnetic Materials, vol. 321, no. 6, pp. 572–577, 2009.
- S. Lan, X. Wu, L. Li, M. Li, F. Guo, and S. Gan, “Synthesis and characterization of hyaluronic acid-supported magnetic microspheres for copper ions removal,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 425, pp. 42–50, 2013.
- B. F. Senkal, F. Bildik, E. Yavuz, and A. Sarac, “Preparation of poly(glycidyl methacrylate) grafted sulfonamide based polystyrene resin with tertiary amine for the removal of dye from water,” Reactive and Functional Polymers, vol. 67, no. 12, pp. 1471–1477, 2007.
- D. Horák, M. Trchová, M. J. Beneš, M. Veverka, and E. Pollert, “Monodisperse magnetic composite poly(glycidyl methacrylate)/La0.75Sr0.25 MnO3 microspheres by the dispersion polymerization,” Polymer, vol. 51, no. 14, pp. 3116–3122, 2010.
- W. Lequieu and F. E. Du Prez, “Segmented polymer networks based on poly(N-isopropyl acrylamide) and poly(tetrahydrofuran) as polymer membranes with thermo-responsive permeability,” Polymer, vol. 45, no. 3, pp. 749–757, 2004.
- G. Kali, S. Vavra, K. László, and B. Iván, “Thermally responsive amphiphilic conetworks and gels based on poly(N -isopropylacrylamide) and polyisobutylene,” Macromolecules, vol. 46, no. 13, pp. 5337–5344, 2013.
- J. Han, K. Wang, D. Yang, and J. Nie, “Photopolymerization of methacrylated chitosan/PNIPAAm hybrid dual-sensitive hydrogels as carrier for drug delivery,” International Journal of Biological Macromolecules, vol. 44, no. 3, pp. 229–235, 2009.
- C. Yang, Y. Guan, J. Xing, G. Jia, and H. Liu, “Synthesis and protein immobilization of monodisperse magnetic spheres with multifunctional groups,” Reactive and Functional Polymers, vol. 66, no. 2, pp. 267–273, 2006.
- Y. Tai, L. Wang, J. Gao, W. A. Amer, W. Ding, and H. Yu, “Synthesis of Fe3O4@poly(methylmethacrylate-co-divinylbenzene) magnetic porous microspheres and their application in the separation of phenol from aqueous solutions,” Journal of Colloid and Interface Science, vol. 360, no. 2, pp. 731–738, 2011.
- W. Zhou, J. Li, W. Wei, Z. Su, and G. Ma, “Effect of solubilization of surfactant aggregates on pore structure in gigaporous polymeric particles,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 384, no. 1–3, pp. 549–554, 2011.
- N. Yanase, H. Noguchi, H. Asakura, and T. Suzuta, “Preparation of magnetic latex particles by emulsion polymerization of styrene in the presence of a ferrofluid,” Journal of Applied Polymer Science, vol. 50, no. 5, pp. 765–776, 1993.
- T.-H. Chung, H.-C. Pan, and W.-C. Lee, “Preparation and application of magnetic poly(styrene-glycidyl methacrylate) microspheres,” Journal of Magnetism and Magnetic Materials, vol. 311, no. 1, pp. 36–40, 2007.
- J. Huang, X. Yuan, X. Yu, and H. Zhang, “Dispersion copolymerization of methyl methacrylate and acrylic acid in polar media: effects of reaction parameters on the particle size and size distribution of the copolymer microspheres,” Polymer International, vol. 52, no. 5, pp. 819–826, 2003.
- E. B. Altintaş, L. Uzun, and A. Denizli, “Synthesis and characterization of monosize magnetic poly(glycidyl methacrylate) beads,” China Particuology, vol. 5, no. 1-2, pp. 174–179, 2007.
- S. A. Hanifah, N. Hamzah, and L. Y. Heng, “Rapid synthesis of magnetic microspheres poly(Glycidyl Methacrylate-co-Styrene) by photopolymerization,” Sains Malaysiana, vol. 42, no. 4, pp. 487–493, 2013.
- E. B. Altintaş, N. Tüzmen, N. Candan, and A. Denizli, “Use of magnetic poly(glycidyl methacrylate) monosize beads for the purification of lysozyme in batch system,” Journal of Chromatography B: Analytical Technologies in the Biomedical and Life Sciences, vol. 853, no. 1-2, pp. 105–113, 2007.
- J. Dou, Q. Zhang, M. Ma, and J. Gu, “Fast fabrication of epoxy-functionalized magnetic polymer core-shell microspheres using glycidyl methacrylate as monomer via photo-initiated miniemulsion polymerization,” Journal of Magnetism and Magnetic Materials, vol. 324, no. 19, pp. 3078–3082, 2012.
- N. Shamim, L. Hong, K. Hidajat, and M. S. Uddin, “Thermosensitive polymer (N-isopropylacrylamide) coated nanomagnetic particles: preparation and characterization,” Colloids and Surfaces B: Biointerfaces, vol. 55, no. 1, pp. 51–58, 2007.
- D. Horák, E. Pollert, and H. MacKová, “Properties of magnetic poly(glycidyl methacrylate) and poly(N-isopropylacrylamide) microspheres,” Journal of Materials Science, vol. 43, no. 17, pp. 5845–5850, 2008.
- L. Lei, X. Liu, Y. Li, Y. Cui, Y. Yang, and G. Qin, “Study on synthesis of poly(GMA)-grafted Fe3O4/ SiOX magnetic nanoparticles using atom transfer radical polymerization and their application for lipase immobilization,” Materials Chemistry and Physics, vol. 125, no. 3, pp. 866–871, 2011.
- J. M. Jin, J. M. Lee, M. H. Ha, K. Lee, and S. Choe, “Highly crosslinked poly(glycidyl methacrylate-co-divinyl benzene) particles by precipitation polymerization,” Polymer, vol. 48, no. 11, pp. 3107–3115, 2007.
- R. G. Sousa, W. F. Magalhães, and R. F. S. Freitas, “Glass transition and thermal stability of poly(N-isopropylacrylamide) gels and some of their copolymers with acrylamide,” Polymer Degradation and Stability, vol. 61, no. 2, pp. 275–281, 1998.
- R. Pierson, C. Basavaraja, N. R. Kim, E. A. Jo, and D. S. Huh, “Microstructure and electrical Properties of poly-N-isopropylacrylamide-N-vinylcarbazole copolymers,” Bulletin of the Korean Chemical Society, vol. 30, no. 9, pp. 2057–2060, 2009.
- N. P. Bayramgil, “Thermal degradation of [poly(N-vinylimidazole)-polyacrylic acid] interpolymer complexes,” Polymer Degradation and Stability, vol. 93, no. 8, pp. 1504–1509, 2008.
- V. V. Khutoryanskiy, “Hydrogen-bonded interpolymer complexes as materials for pharmaceutical applications,” International Journal of Pharmaceutics, vol. 334, no. 1-2, pp. 15–26, 2007.
- D. López, I. Cendoya, F. Torres, J. Tejada, and C. Mijangos, “Preparation and characterization of poly(vinyl alcohol)-based magnetic nanocomposites. 1. Thermal and mechanical properties,” Journal of Applied Polymer Science, vol. 82, no. 13, pp. 3215–3222, 2001.
- G. Török, V. T. Lebedev, L. Cser, and M. Zrinyi, “NSE-study of magnetic phase dynamics in poly(vinylalcohol) ferrogel,” Physica B: Condensed Matter, vol. 276–278, pp. 396–397, 2000.
- Z. Varga, J. Fehér, G. Filipcsei, and M. Zrínyi, “Smart nanocomposite polymer gels,” Macromolecular Symposia, vol. 200, no. 4, pp. 93–100, 2003.
- L. Liang, X. Feng, L. Peurrung, and V. Viswanathan, “Temperature-sensitive membranes prepared by UV photopolymerization of N-isopropylacrylamide on a surface of porous hydrophilic polypropylene membranes,” Journal of Membrane Science, vol. 162, no. 1-2, pp. 235–246, 1999.
- E. S. Abrutyn, R. C. Chromecek, and L. J. Scarfo, “Lattice-Entrapped Composition,” Google Patents, 1988.
- G. Bayramoğlu, M. Yılmaz, A. Ü. Şenel, and M. Y. Arıca, “Preparation of nanofibrous polymer grafted magnetic poly(GMA-MMA)-g-MAA beads for immobilization of trypsin via adsorption,” Biochemical Engineering Journal, vol. 40, no. 2, pp. 262–274, 2008.
- E. Pollert, K. Knížek, M. Maryško et al., “Magnetic poly(glycidyl methacrylate) microspheres containing maghemite prepared by emulsion polymerization,” Journal of Magnetism and Magnetic Materials, vol. 306, no. 2, pp. 241–247, 2006.
- G. Senanayake and G. K. Das, “A comparative study of leaching kinetics of limonitic laterite and synthetic iron oxides in sulfuric acid containing sulfur dioxide,” Hydrometallurgy, vol. 72, no. 1-2, pp. 59–72, 2004.
- C. Bergemann, D. Müller-Schulte, J. Oster, L. à Brassard, and A. S. Lübbe, “Magnetic ion-exchange nano- and microparticles for medical, biochemical and molecular biological applications,” Journal of Magnetism and Magnetic Materials, vol. 194, no. 1, pp. 45–52, 1999.
Copyright © 2014 Siti Zulaikha Mazlan et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.